Electronic Supporting Information
Sharp Cu@Sn nanocones on Cu foam for highly selective and
efficient electrochemical reduction of CO2 to formate
Chengzhen Chena, Yuanjie Pangb, Fanghua Zhanga, Juhua Zhongc, Bo Zhang*d and Zhenmin
a State Key Laboratory of Chemical Engineering, School of Chemical Engineering, East China
University of Science and Technology, Shanghai 200237, China.
b School of Optical and Electronic Information, Huazhong University of Science and
Technology, Wuhan, Hubei 430074, China.
c Department of Physics, East China University of Science and Technology, Shanghai 200237,
d State Key Laboratory of Molecular Engineering of Polymers, Department of Macromolecular
Science, Fudan University, Shanghai 200438, China.
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.This journal is © The Royal Society of Chemistry 2018
Supplementary figures and tables
Table S1. The bulk pH of aqueous electrolytes after CO2 saturation.
Electrolytes Bulk pH after CO2 saturation
0.1 M KHCO3 6.83
0.05 M KCl+0.1 M KHCO3 6.80
0.1 M KCl+0.1 M KHCO3 6.79
0.2 M KCl+0.1 M KHCO3 6.77
0.3 M KCl+0.1 M KHCO3 6.76
Fig. S1 (a) Low-magnification and (b) high-magnification SEM images of the Cu foil after
Fig. S2 Chronoamperometry curve for the electrodeposition of Cu-Ni nanocones precursor on
Fig. S3 Chronoamperometry curve for the electrodeposition of Cu-Ni nanocones precursor on
Fig. S4 Schematic illustration of a two-compartment electrolysis cell.
Fig. S5 (a) 1H-NMR spectrum for a standard formate sample (4 mM); (b) the linear relationship
between the standard formate concentration and relative area vs. TMSP. The relative areas were
estimated by following equation:
Relative area (formate) = peak area at 8.45 ppm (formate)peak area at 0.00 ppm (TMSP)
Fig. S6 Energy-dispersive X-ray spectra of Cu-Ni nanocones precursor on Cu foil.
Fig. S7 High-resolution XPS spectra for the Ni 2p region of Cu-Ni nanocones.
Fig. S8 (a) Low-resolution and (b) high-resolution SEM images of Cu-Ni nanocones precursor
on Cu foil.
Fig. S9 Potential curve for the deposition of Sn on the Cu nanoconic surface at a constant current
density of 3.3 mA cm-2 to prepare the Cu@Sn nanocones.
Fig. S10 XPS survey spectra of Cu nanocones.
Fig. S11 (a) Low-resolution and (b) high-resolution SEM images of Cu nanocones precursor.
Fig. S12 SEM image of a small amount of bulk Sn lying above the Cu@Sn nanocones layer.
Fig. S13 Cyclic voltammogram curves (scan rate: 20 mV s-1) in N2 or CO2 saturated 0.1 M
KHCO3 electrolyte of (a) Cu nanocones, (b) Cu@Sn nanocones with Sn deposition time of 800 s,
(c) bulk Sn.
Fig. S14 Effect of Sn deposition time on formate faradaic efficiency with Cu@Sn nanocones at -
To optimize the electrocatalytic performance, Cu@Sn nanocones electrodes differing in the Sn
deposition time were prepared and subsequently tested at -0.9 V in CO2-saturated 0.1 M KHCO3.
The gaseous product and liquid product were determined using gas chromatography (GC) and
NMR spectrometer, respectively. Interestingly, the formate faradaic efficiency rose significantly
with prolonging the Sn deposition time, reaching a maximum value of 67.6% at deposition time
of 800s (Fig. S14), and then decreased with further elongating the time to 1400s, accompanied
with the increased density of bulk Sn above the nanocones layer (Fig. S15). Thus, the Cu@Sn
nanocones with tin deposition of 800s was used for all physical characterization and labelled as
Cu@Sn nanocones on the whole work.
Fig. S15 SEM images of Cu@Sn nanocones with various Sn deposition time of (a) 200 s, (b)
700 s, (c) 900 s, (d) 1400 s.
Fig. S16 Total current density of Cu nanocones at various potentials measured in CO2-saturated
0.1 M KHCO3.
Fig. S17 (a) TEM image, (b) SEM-EDS mapping of Cu@Sn nanocone after electrolysis; (c)
XRD patterns, (d) Sn 3d 5/2 XPS spectra of Cu@Sn nanocones and Sn particles after electrolysis.
After CO2 electrolysis, the conical structure of Cu@Sn nanocones was retained, with deposited
Sn well preserved (Fig. S17a and S17b). Meanwhile, no other peaks were observed in the XRD
data except for the peaks of bulk metallic copper and tin ((JCPDS 86-2265)) (Fig. S17c), while
the exposure of surface Sn to air before XPS measurements led to the spontaneous and partial
oxidation (Fig. S17d).
Fig. S18 Faradaic efficiency of different products on Cu nanocones at various applied potentials.
Fig. S19 Formate partial current density of Cu@Sn nanocones and bulk Sn at various potentials.
Fig. S20 (a) Cu@Sn nanocones, (b) Sn particles charging current density plotted against various
CV scan rates; (c) double layer capacitance plots. The electrochemical surface area (ECSA) was
estimated from the double-layer capacitance (Cdl) of different catalysts in N2-satarated 0.1 M
KHCO3. Cyclic voltammetry was record in a potential window where only double layer charging
and discharging happened. Plotting the △j/2 ((ja-jc)/2) at the middle point of potential window
against CV scan rates would acquire the Cdl, where ja and jc are the corresponding anodic and
cathodic current density.
Fig. S21 Formate faradaic efficiency of Cu@Sn nanocones in different electrolytes.
The CO2 reduction on Cu@Sn nanocones in 0.1 M KCl electrolyte were also performed (Fig.
S21). It shows that formate faradaic efficiency (FE) was slightly decreased in the KCl electrolyte
compared to that in KHCO3 solution. A similar phenomenon also has been observed in
nanostructured Ag catalyst.1
To get a better focus on Cl- and eliminate the beneficial effect of K+, CO2 experiments on
Cu@Sn nanocones were carried out in 0.1 M NH4Cl electrolyte. The results show that formate
FE was dramatically declined only with the presence of Cl- (Fig. S21).
These results together confirm that the increament of K+ concentration was responsible for the
improved formate selectivity in Fig. 4e
Fig. S22 Nyquist plots of Cu@Sn nanocones in CO2-saturated electrolyets in a frequency range
from 1 MHz to 0.05 Hz with 10 mV amplitude at -0.95 V vs. RHE
Fig. S23 (a) Low-magnification and (b) high-magnification SEM images of Cu foam substrate.
Fig. S24 (a) Low-magnification and (b) high-magnification SEM images of Cu-Ni nanocones
precursor over Cu foam.
Fig. S25 SEM-EDS mapping results of Cu@Sn nanocones/Cu foam catalysts.
According to the ratio of average current density in depositing Cu-Ni nanocones on Cu foam
relative to Cu foil (Fig. S2 and Fig. S3), the deposition time of Sn was prolonged to 2100 s for
Cu@Sn nanocones/Cu foam electrode.
Fig. S26 (a) Low-magnification and (b) high-magnification SEM images of Cu@Sn nanocones
catalyst after 10 h reaction.
Table S2. Comparison of the electrocatalytic performance of noble-metal-free Sn-based catalysts.
Cu@Sn nanocones/Cu foam 0.1 M KHCO3+0.3M KCl -1.10 90.4 57.7
Cu@Sn nanocones/Cu foil 0.1 M KHCO3 -1.10 88.4 20.4 80.1 This work
SnO2 nanosheets/carbon cloth 0.5 M KHCO3 -0.95 89 48.6 79 Li et al.2
Sn particle/carbon nanotube areogel
0.5 M KHCO3 -0.96 82.7 26.7 155 Chen at al.3
Nanoporous tin foam 0.1 M NaHCO3 -1.30 90 23.5Not
studiedDu et al.4
Metallic tin quantum sheets 0.1 M NaHCO3 -1.15 89 21.1 83 Lei et al.5
Tin dendrite 0.1 M KHCO3 -1.36 71.6 17.1 145 Won et al.6
SnS2 nanosheets 0.5 M NaHCO3 -0.8 84.5 13.9 83 Li et al.7
SnO2 nanoparticles 0.1 M NaHCO3 -1.15 93.6 10.2 70 Zhang et al.8
SnO2 porous nanowires 0.1 M NaHCO3 -1.0 76 10 134 Kumar et al.9
Porous tin film 0.1 M KHCO3 -1.2 91.5 5.5Not
studiedLu et al.10
Thin SnOx/Sn layer 0.1 M KHCO3 -1.09 77.4 4.8 146 Daiyan et al.11
Deposited Sn particles 0.1 M KHCO3 -1.15 63 4.5 169 Zhao et al.12
Sn foil 0.5 M NaHCO3 -0.7 0.3 3 74 Chen et al.13
[a] Applied potential at the maximum faradaic efficiency. [b] Maximum faradaic efficiency.
[c] Total current density at the maximum faradaic efficiency.
1.S. Verma, X. Lu, S. Ma, R. I. Masel and P. J. Kenis, Phys. Chem. Chem. Phys., 2016, 18,
2. F. Li, L. Chen, G. P. Knowles, D. R. MacFarlane and J. Zhang, Angew. Chem. Int. Ed., 2017,
3. Z. Chen, S. Yao and L. Liu, J. Mater. Chem. A, 2017, 5, 24651-24656.
4. D. Du, R. Lan, J. Humphreys, S. Sengodan, K. Xie, H. Wang and S. Tao, Chemistryselect,
2016, 1, 1711-1715.
5. F. Lei, W. Liu, Y. Sun, J. Xu, K. Liu, L. Liang, T. Yao, B. Pan, S. Wei and Y. Xie, Nat.
Commun., 2016, 7, 12697.
6. H. Won da, C. H. Choi, J. Chung, M. W. Chung, E. H. Kim and S. I. Woo, ChemSusChem,
2015, 8, 3092-3098.
7. F. Li, L. Chen, M. Xue, T. Williams, Y. Zhang, D. R. MacFarlane and J. Zhang, Nano Energy,
2017, 31, 270-277.
8. S. Zhang, P. Kang and T. J. Meyer, J. Am. Chem. Soc., 2014, 136, 1734-1737.
9. B. Kumar, V. Atla, J. P. Brian, S. Kumari, T. Q. Nguyen, M. Sunkara and J. M. Spurgeon,
Angew. Chem. Int. Ed. , 2017, 56, 3645-3649.
10.W. Lv, J. Zhou, F. Kong, H. Fang and W. Wang, INT J HYDROGEN ENERG, 2016, 41,
11. R. Daiyan, X. Lu, Y. H. Ng and R. Amal, Catal. Sci. Technol., 2017, 7, 2542-2550.
12. C. Zhao and J. Wang, Chem. Eng. J., 2016, 293, 161-170.
13. Y. Chen and M. W. Kanan, J. Am. Chem. Soc., 2012, 134, 1986-1989.